Review on carbon nanomaterials as typical candidates for orthopaedic coatings
- 348 Downloads
Implants are frequently administered devices to provide mechanical support to restore the function of diseased tissues and supports the natural healing process. The new concept of coated implants come to exist after 1980s to overcome the limitations related to prosthetic failures. The hurdles such as corrosion, infection and lack of bone integration of implant are the primary culprits for the failures. The present review provides a deep insight about the carbon nanomaterials (CBNs) as potential candidates for implant coatings. Additionally, the document highlights the limitations of pristine materials and discusses the different modalities to resolve the issues. The unique structural, thermal, mechanical and electrical properties of CBNs have been presented in detail to understand the significant utilization of CBNs in biomedical sciences and technology. The review may provide an opportunity for researches to develop novel materials for futuristic applications.
KeywordsCarbon nanomaterials Orthopaedic implant Coatings Osteoconductive Antibacterial Corrosion resistance
Joint replacement is major surgical intervention to treat the severe damage of articular surfaces, due to cancer deformities of musculoskeletal tissues and distortions by various mechanical interferences. The procedure involves the replacement of total joint or part of joint by the prosthesis. The most common articular damage is osteoarthritis and it is mainly characterized by the degradation of bone, pain and deformity . The first successful joint replacement attempt is recorded in 1948 at New York orthopedic hospital. About 2.2 million bone surgeries are taken place every year to get rid of the condition . The articular joint prosthesis is a device, which restores the function of the joint by providing mechanical support or complete replacement of skeletal tissue. Generally, the devices are made up of metals, ceramics, plastics/polymers and composites. Traditionally, various metals have been practiced in healthcare particularly on orthopaedics, such as lead, silver, aluminum, iron, copper and zinc etc. Despite their adverse effects towards the biological system, due to lack of technology advancement. In modern medical technology, several bio-friendly materials/metals are successfully employed in complex surgeries. The metals like stainless steel, zirconium, titanium and their alloys are largely used in orthopaedics, since the late 1930s . Predominantly, stainless steel, cobalt chrome alloy, titanium and their alloys are mostly utilized for musculoskeletal applications, due to their good biocompatibility, high corrosion resistance, extraordinary mechanical strength and low cost .
Regardless of the great progress of medical implants technology and it is suffered from a set of limitations to restrict the success rate up to some extent. Frequent issues related to orthopedic implants like corrosion, loosening of the device; due to poor mechanical strength, infection, non- integration of implant with host tissue and wearing are the prime factors of concerns [19, 31, 87]. The far most characteristic of an orthopedic implant is integration to host tissue to boost the success rate by resisting the colony formation of microbes and corrosion .
Infections of fracture-fixation devices involve complex treatment with a 6-week course of systemic antibiotics and it requires less time interval (15 days) for superficial infections . In many cases, the infections lead to the failure of the prosthesis and require the revision of surgery . The coating on the implant is come to exist to avoid the infection  and corrosion related failures; further, the bioactive coatings largely enhance the integration to the host tissues .
The coating is a specific material cover on the surface of the implant system with predefined thickness. In general, the objective of the coating is to protect the implant from corrosion, infection, friction, promote the osteoconductivity and osseointegration. Interaction at the interface of the implant and surrounding tissue is a key factor in the success of implant and where coating plays a vital role. The ideal properties of coating material is non-toxic, non-carcinogenic, non-immunogenic and non-thrombogenic  and it is very difficult to find all ideal characteristics in a single coating material/formulation. Coatings in dentistry have been reported since 1970’s but orthopedics follows the footsteps quite late in the 1980’s. First coated implantation is taken place at St Thomas Hospital in London in 1981 .
Design of coating material is challenging research and it has to full fill certain measures. Firstly, it should be biocompatible and non-immunogenic; second, it must have sufficient mechanical strength and should form a mechanical bond to the host tissue to withstand, when functional stress occurs. Third, it has to be osteoconductive to promote the integration of the host tissue and it should possess osteoinductive to differentiation of recruited stem cells into osteogenic cells from surrounding tissues. Finally, the coating material should hold an antimicrobial activity to avoid the failure of implant system by post-surgery infection. None of the current commercial implants or coatings possess all required properties . Therefore, there is a need for further research on biological coatings, which fulfill the maximum benchmarks and improves the life of the implant.
Adequate research is available on orthopedic coating material such as Hydroxyapatite (HA) [29, 42, 73, 120]. HA attracts more to the researchers as its chemical composition similar to natural bone. Moreover, HA is highly biocompatibility and osteoconductive, hence it is quite suitable for orthopedic applications. Collagen and collagen-based composites are used mostly in regenerative medicine but poor mechanical properties limit their usefulness in hard tissue applications [14, 38, 52, 56, 64]. Bioglass [12, 70, 84, 92] is an attractive alternative, since, it promotes proliferation of bone tissue much faster as compared to healing occur in autogenously bone graft and HA . Furthermore, it has been well documented that the bioglass stimulates the angiogenesis and offer antibacterial effect . Despite, its benefits, bioactive glass is still in limited usage by its high elastic modulus. Polymers  are used for coatings, such as polycaprolactone (PCL) [48, 117], poly-D L lactide [27, 119], polyurethane , polyaniline and polyimide, which shows high anti-corrosive and good cell differentiation properties. Apart from composites of synthetic polymers, the composites of natural polymer like cellulose, starch and acetate with HA were well demonstrated for enhanced osseointegration [74, 88, 89, 116]. Antibacterial and osteoconductive drug molecules are also used for various coatings [96, 111]. Particularly, drugs like simvastatin are used to enhance cell growth and callus formation, whereas antibiotics like gentamicin and ciprofloxacin are used to inhibit post-surgical infections . The key role of the coating to provide control release of the drug, else it leads to drug-related toxicity from uncontrolled release [51, 119]. In alternative, growth factors such as Bone-Morphogenetic Protein (BMP-2), Platelet-derived Growth Factor (PDGF), Transforming growth factor (TGF) and Vascular Endothelial Growth Factor (VEGF) are generally administrated through polymers to enhancing the bioactivity of the coating, however, these limits by uncontrolled growth of tissues and high cost [51, 75].
The contemporary researchers are trying to avoid all adverse effects of implants by adopting nanotechnology and explore new-engineered materials of a natural source. Carbon is an extraordinary material for various applications and it is available in various forms with a range of properties. It has been being used extensively in aerospace, electrical, electronics and energy generation applications, but limited in biology. Carbon is discovered in prehistory and has been known since the ancient period. Naturally occurred carbon source such as amorphous carbon, graphite and diamonds are in allotropic in nature. Engineered carbon structures like nanotubes (CNT) and fullerenes are also in allotropic of carbons. Sumio ljima et al. reported fiber form of carbon structure in 1991, known as CNT and it possesses significant mechanical, thermal and electrical properties . Whereas, fullerene is much stable carbon structure, since its graphite-like bonds . The sheet-like graphene is single layer carbon source and it is the building block of all allotropes, when it is stacked to 3D it forms 3D graphite, rolled to form 1D CNT and wrapped to form 3D fullerene . Significantly, nano-sized carbon sources were well demonstrated in augmented properties in various aspects such as mechanical, electrical, thermal and physical properties . The enhanced properties of the nano-sized materials come from its unique structures and atomic alterations . The first study in biomedical on nano-carbon for osteoblast differentiation is reported by Webster and co-workers in 2002. The study was reported with increased osteoblast proliferation, alkaline phosphatase activity, and bone mineral deposition on carbon nanofibers than micron-sized fibers and titanium implants . Carbon is an important material for biological applications by its succeeding motives; it improves the level of osseointegration, since, hybrid of microscale pits in implant surface and layers of sheets or tubes mimic the cellular environment thus enhances the rate of integration. It shows excellent antimicrobial activity: due to its ordered structure and strong mechanical properties, CNTs are stronger than steel. Even more the graphene is stronger than all carbon derivatives including diamond . Though, graphene is the strongest material, it is lightest and thinnest material ever found . Fullerenes are commonly known as ‘Buckyball’ (C60). It is a spherical cage-like structure which is made up of sixty sp2 carbons and discovered in 1985 . Further, it shows unique electronic properties from its stemming symmetrical structure. Exploring various applications of CBN starts with the discovery of C60. Fullerene is not much accepted in orthopedics because of the discovery of more practical carbon-based materials like CNT and graphene. However, it shows anti-HIV activity .
However, some challenges limit the use of CNTs in real-world applications. Primarily, the cytotoxicity is the major hurdle, due to residual impurities during synthesis . Impurities like amorphous carbon, residuals of catalytic particles are highly disturbed the living environment. Even more, the purification strategies also introduce cytotoxic substances in certain cases (e.g. sodium dodecyl sulfate) . Kaiser et al. have identified high oxidative stress generated when CNTs interact with cells and initiates the oxidative stress-responsive pathway, which releases pro-inflammatory cytokines such as IL. Most of the in vivo studies reveal that, a high concentration of CNT causes changes in cell and tissue morphology [4, 118]. Beside, CNT causes acute toxicity . Therefore, proper modification or alteration of pristine materials are highly necessary to reduce the adverse effects in biological use.
As mentioned, CNTs toxicity is mainly caused by synthesis residues such as heavy metals like nickel, cobalt, nickel-aluminum alloy . Alternatively, graphene can be synthesized in relatively pure form and thereby decreases the risk of toxicity . Graphene was first isolated by Novoselov and Geim in 2004 and it is a one-atom thin sheet of carbons and arranged in a 2D honeycomb-like structure . The aromatic structure of graphene contains a crowd of free π-electrons and presence at each atom. The unique structural features of graphene possesses, excellent properties like large specific surface area, high Young’s modulus (1TPa), high electron mobility, and high thermal conductivity and impermeability to gases . Geim and Novoselov reported a simple method for the extraction of graphene from graphite via chemical exfoliation and research on graphene is still in an infancy stage particularly for the biomedical application .
Graphene oxide (GO) is an oxidized derivative of graphene. GO has a number of reactive oxygen functional group like epoxy, carboxylic and hydroxylic group . Because of its derivatization GO become more biocompatible, hydrophilic in character and interacts easily with protein via covalent, hydrogen and electrostatic bonding . The GO is more suitable for medical application than graphene, since its low toxicity, better dispersion in an aqueous medium, the presence of a large number of functional groups enables it react with various substrates and GO has a wide range of physical properties than pristine graphene .
Hamed et al. reported a study on morphological change and its effect on mechanical properties of graphite carbon nanoparticles (GCNs) embedded epoxy resin composite. The study was carried out with variable concentrations of GCNs from 1 to 5 wt% in epoxy resin. The team reported that relatively short and agglomerated morphology in 5 wt% as compared to 2 wt%. Interestingly the 2 wt% composite was shown enhanced hardness (12.5%) and modulus (8%) as compared to the pristine epoxy, while the 5 wt% composite shows nearly same properties as pristine epoxy. The same trend was reported in tensile and compressive properties for 2 and 5 wt% composites. The suggested reason is stress concentration is higher in an epoxy matrix surrounded by a rod-shaped particle as opposed to round or elliptical particles and stress concentration effect rising from 1 to 5 wt% composites. Therefore the concentration optimization of CBN is a key parameter to achieve enhanced properties in coating technology .
2 CBNs as orthopaedic coatings
2.1 Osteoconductive coatings
From last decade, CBNs are greatly exploring in the biomedical arena, due to its significant characters and keenly monitoring its toxicity. CNT accelerates the precipitation of calcium phosphate (CaP), due to the presence of more nucleation centers for crystal nucleation and growth . The phenomenon is known for, when bone is subjected stress, it generates an electrical signal to bone remodeling thereby regulates the bone regeneration and bone healing [41, 77, 104]. Therefore, CNT contained scaffold can be used for stimulating the cell growth and tissue regeneration by facilitating the physioelectrical signal transfer as CNTs are good electric and thermal conductor . Further, to fasten the bone healing and to improve the surface bioactivity Ning CAO reinforces the CNT in HA and enhanced osteoconductive was observed against pristine carbon fibers. The study was carried out in goat model for 18 months, calcium and phosphorus ions leached from HA to provide suitable biological mineralization which accelerates the osteoblast differentiation and collagen synthesis.
Several polymers are well bioactive but inferior in mechanical properties limit its use in tissue engineering. X. Shi. et al. fabricated on SWCNT reinforced poly (propylene fumarate) (PPF) nanocomposite. Significantly, the functionalized CNTs are shown improved dispersion in PPF over pristine CNTs . Titanium (Ti) is commonly used implant material for dental applications because of its biocompatibility and high Young’s modulus . Various surface modification (e.g. apatite coat, anodization) were employed over titanium to achieve early integration of bone tissues. Saori Inoue and co-workers investigated on the MWCNT based coating on anodized titanium implant. The Human osteosarcoma cells (SaOS2) are cultured with CNT-Ti disks and reported high proliferation rate as compared to HA. Even more, the DNA content of cells on CNT-Ti is significantly higher than simple HA coating after 7 days of incubation. Furthermore, enhanced bone contact ratio with CNT-Ti against HA is reported in an animal model .
Various carbon forms and their major composite used in osteoconductive coating
Carbon-based nanomaterials CBN)
CNT + HA
Apatite formation depends on –COOH group attached to CNT
CNT + HA + TiO2
Enhances pre-osteoblast formation and proliferation
CNT + Anodized Ti
DNA quantification shows higher cell count in CNT + Anodized Ti than simple Ti coating
CNT + Chitosan
Scaffold shows good biocompatibility and remarkable osteoblast terminal differentiation(7 days)
CNT + PCL + nAg
The composite shows synergistic effect on both antibacterial and conductivity
Uniform layer of osteoblasts are formed after 48 h incubation
Graphene + Ag
Well established for antibacterial and Osteoconductivity
Graphene + GO + CaCO3
GO/Graphene–CaCO3 composite intensifies the formation of HA, compared to bare GO or graphene
GO + HA + PLA
30% w/w HA and 1% GO shows high mechanical strength and osteoblast differentiation
GO + PCL/PLGA
PCL and PLGA nanofiber membrane provide strong, porous and bioactivity
GO + Collagen
Higher tissue growth in collagen coating than non-coated scaffold but less than rGO-collagen
rGO + Collagen
Calcium adsorption and alkaline phosphatase activity enhanced due to presence of rGO
rGO + HA
Enhanced mechanical properties and in-vitro cell activity
Reduced graphene oxide (rGO) obtained by various methods of UV, thermal and chemical treatment of GO under the reducing condition with reducing agents like hydrazine . Izumi and co-workers have done a comparative study of the bioactivity of GO and rGO. GO and rGO are coated onto collagen scaffold, implanted into rats back and characterized by SEM. DNA content and cell ingrowths of the implanted scaffold are measured after 10 days of surgery. The compressive strength of GO and rGO coated collagen scaffold is increased by 1.7 fold and 2.7 fold greater than the non-coated scaffold. Tissue growth rate is 39% in rGO and 20% in GO coated scaffolds. Result clearly indicates that rGO is more bioactive than GO . rGO–HA composite is found to be enhanced mechanical property along with the improved proliferation and alkaline phosphatase (ALP) activity of human osteoblastic cells. HA-rGO nanocomposite is synthesized by liquid precipitation method . In these way various carbon forms play a role as osteoconductive and hence recently researcher attracted more towards carbon nanomaterials for biomedical applications.
Another potent carbon contender for osteoconductive coatings is nano-diamond. The Recent in vivo study has been confirmed that, the nano-crystalline diamond (NCD) promotes intense bone growth, than micro-crystalline after 4 and 8 weeks. The nano-diamond also possess antioxidant, anti-inflammatory, anticancer and anti-allergic properties . Though, a mechanism for osteoconductivity is not clear, but it is assumed that the osteoblast filopodial extension and cytoskeleton spreading are mechanically affected due to geometry and size of the surface features on NCD which lead to elevated cell proliferation and differentiation .
2.2 Antibacterial coatings
Hybrid CNTs with polymers and different metal ions (e.g. Copper, Silver) find to be more effective than pristine CNT to inhibit the microbial attachment and colony formation . Interestingly, Kang et al.  reported that SWCNT is more toxic than MWCNT to the bacteria as the diameter of CNT plays a major role in anti-bacterial activity. S. Liu and co-workers studied the effect of pristine SWCNT dispersion in media. The homogeneously dispersed CNTs have shown greater antibacterial activity than in aggregate form and the effect is examined by colony formation count and viability assay method. Furthermore, the study reveals that the dispersed SWCNT shows higher antibacterial property towards gram-positive bacteria than gram-negative . However, purification process of CNT is very tedious and the residual fragments are primarily responsible for cell toxicity. Therefore, research focuses more on functionalization or surface medication to reduce the toxicity of pristine CNTs. From the bingeing, silver (Ag) is well established for its anti-bacterial applications. The action comes from its strong interaction with protein sulfhydryl group, which founds in cell wall and cytoplasm thereby affects the metabolic activity . M. Prodana and co-workers enhance the anti-microbial activity of functionalized MWCNT by using silver nanoparticle. Silver nanoparticles are attached to the surface of functionalized MWCNT (MWCNT-COOAg) by simple electrostatic adsorption. The result shows that CNT enhances percentage inhibition of E. Coli growth from 19 to 34% and it is better than a pristine silver nanoparticle. Further, MWCNT-COOAg enhances the percentage inhibition from 34 to 68% . A similar study was reported by Aping Niu and group, in which CNTs are wrapped with silver nanoparticles. The research shows that, CBN exhibit good antibacterial property against E-coli and inhibits bacterial growth higher than 0.5% . Copper (Cu) is ranked second after Ag in terms of antibacterial property and it is stable and non-toxic in a physiological environment. Pandey et al.  reported that CNT with ceria and silver nanoparticle incorporated HA coating on the Ti-implant enhances the cell adhesion as well as significantly inhibit the growth of E-coli. The most common infection at the site of implant prosthesis is Staphylococcus epidermidis. Hirschfeld et al.  demonstrated MW-CNT impregnated with the rifampicin coated on the TiAl6V4 implant study reveals that the MW-CNT coated implant synergistically inhibit the biofilm formation as well as it helps in controlling the release pattern of rifampicin. Liu et al.  reported that Cu coated CNT has higher antibacterial activity than the Cu coated pyrolytic carbon and the suggested reason is CNT offers a higher surface area for Cu deposition than pyrolytic carbon. Wenbing Hu et al. synthesized antibacterial GO sheet by modified Hummer method with low cytotoxicity than CNT. GO demonstrates the excellent antibacterial activity and significantly suppressed the viability of E-coli up to 98.5%. Reduced graphene oxide is also showed antibacterial activity and decreases the metabolic activity of E-coli about 24% . Ghosh et al. synthesized a GO-Para Amino Benzoic Acid (PABA) nanosheets by modified chemical exfoliation of graphite. The GO-PABA-Tetracycline hybrid nanosheet shows good biocompatibility, high drug loading efficiency and good antibacterial activity . Pandey et al. rise the antibacterial effect of graphene nanosheet by loading of gentamicin sulfate. The study has revealed that graphene is a good matrix to achieve controlled release and diffusion dominated release mechanism .
Hydrogenated diamond-like carbon (DLC) contains the mixture of Graphite and Diamond. It attracts the scientist because of a wide range of structural variation. The study is carried out on pure DLC, metal doped DLC and carbide doped DLC by various scientists. The studies have been revealed that the increased copper content in DLC enhances the antibacterial activity against E. coli and concludes that DLC films are highly suitable for protective material in biomedical field .
2.3 Anticorrosive coatings
Corrosion is a crucial problem associated with metallic implants and it is characterized by oxidization of metal surfaces by chemical or electrochemical interactions. CBN has many remarkable properties as being chemically inert and they can be used as anticorrosive coatings in biomedical applications. The suggested mechanism is that, CNT act as physical barrier for chemical interaction by filling inside the crevices, gaps and holes on the surface of Nickel (Ni) . Corrosive resentence was increased, when the implant is coated with layer by layer technique then bulk coating. The well-dispersed CNT in Ni is coated on steel and demonstrated high corrosive resistance. Besides, the Ni-CNT composite shows good antibacterial activity as well . One interesting study was reported on Ni/P/SWCNT composite for corrosive resistance coatings and corrosion behavior is evaluated by polarization curves in 0.1 M NaCl solution. The Ni/P/CNT composite shows higher corrosion resistance than Ni/P composite by providing more uniform coating . Magnesium is one of the lightest metal but it is more prone to corrosive in biological environment. M. Endo incorporates the MWCNT as filler in magnesium alloy matrix and the hybrid is well demonstrated for corrosion resistance as compared to the magnesium alloy. The matrix of organic (trialkoxysilane and polymethyl methacrylate) and inorganic (Al2O3, ZrO2 and SiO2) nanocomposite with CNT fillers are prepared by various physical and chemical methods and reported as coating materials. Both phases interact by weak intermolecular forces or by a covalent bond in some cases. XPS and TG study show that stability of hybrid network increases due to CNT and thereby showed superior performance in acidic media . Show et al. fabricated a composite film of CNT reinforced in polytetrafluoroethylene. The hybrid has demonstrated with high electrical conductivity and corrosion resistance . Kumar et al. observed the synergistic effect of two nanofillers (CNT and Ag nanoparticle) in the PCL matrix. The study reveals that, PCL-MWNT-nAg nanocomposite improves antibacterial activity, electrical conductivity and resistance to corrosion .
Graphene is well proved anticorrosive material since its high inertness . Raman et al. studied the corrosive properties of graphene coated Cu film in the presence of a very aggressive electrolyte. The film increases impedance significantly and reduced anodic and cathodic current density and thereby protect the metal film from corrosion . A similar study was carried out by Feng Zhou et al. for a longer time at ambient conditions. Here they reported that the graphene coating can accelerate long-term oxidation of copper . Zang et al. prepared a graphene-epoxy hybrid coating and investigated by electrochemical measurement. The study shows a far lower erosion in the hybrid coating (0.3 mm/yr) than neat epoxy resin (1.3 mm/year). Thus, graphene approach not only improves the erosion resistance but also shows high mechanical and thermal properties against pristine epoxy coating . Chang et al. prepared an electroactive polyimide (PI) and graphene nanocomposite (PGN) coating by thermal imidization method. The redox behavior of PGN material is examined by in situ cyclic voltammetry (CV) and the study found that EPGN matrix shows enhanced oxygen barrier property . Reduced graphene oxide is covalently attached over silicon wafers and the coating offers excellent corrosive and wear resistance .
Nitinol has superplastic property and shape memory effect but the toxicity limits its use in health care. Branzoi et al. developed a surface modification method for nitinol to improve its corrosion resistance and biocompatibility. The diamond-like carbon (DLC) has coted over the alloy by magnetron sputtering method. The coating shows improved corrosion resistance and surface hardness. Hence, nitinol with DLC may be a potential candidate for anticorrosive coatings for medical applications .
The advanced properties of CBNs like biocompatibility, osteoconductivity, high mechanical properties, chemical stability, good thermal conductivity and antibacterial activity pit them as a better alternative for coating technology in regenerative medicine. Moreover, high electron density and high volume to surface area of CBN can offer ease of manipulation to tune the desired properties by various simple methodologies such as functionalization, surface modification and doping. Hence, the materials have attracted by the researchers in various fields predominantly, electronics, aerospace, automobile etc. The exploration of CBNs are limited in biomedical and they can give an opportunity to cultivate cutting-edge inventions for futuristic applications. However, pristine materials are well proved in some aspects like mechanical, electrical and thermal, but need to establish in biologically. There is a huge scope in the area of modification of pristine materials to overcome the limited hitches to come as an absolute material for medical applications. Another major field of exploration is the development of simple synthesis methodologies, particularly for biomedical applications the processing residual chemical moieties are primary culprits for cytotoxicity. Importantly, graphene is not yet fully explored for biomedical applications. Therefore, CBNs can give potential opportunities for researchers to novel innovations for biomedical applications.
2.4 Advanced material coating: carbon quantum dots
3 Adverse biological effect of CBN coated implants
As CNT is the most promising material for coatings, but the toxicity limits its applications in biomedical applications. The toxicological profile of CNT was well reviewed by Constantine et al. The CNT induces the oxidative stress and results in DNA damage in organs like liver, lungs and spleen . Nevertheless, very little information is available on the effect of wear debris of CNT. Lahiri et al. carried out wear debris activity of HA-CNT composite coating. The study divulges that debris of HA-CNT composite is not evident for any adverse effect on osteoblast, moreover the wear particles show normal activation of macrophages . While, the graphene demonstrates diverse toxicological profiles and it was well emphasised by Yang et al. The in vitro studies suggest the pristine graphene exhibit poor cell penetration and good biocompatibility. Although some reports advocate that graphene shows a negative effect on cell via inducing oxidative stress, ROS generation and alteration of expression of key genes and proteins . However, no productive report was found to understand the effect of wear debris and leaching of graphene coated implants.
The scientific community is reporting extensive work on CBN coatings for orthopedic applications. The current review introduced deep insight of various applications of CBNs in orthopedic coatings, which can also use in other biomedical coatings. The document presents the special glimpse on the novel carbon material like Carbon quantum dots for hard tissue applications. CBN’s offer versatile property like biocompatibility, unique surface, electrical, chemical, mechanical and thermal properties of the other advanced materials. Hence, CBNs can expect to see a continuous rise in utilization in the biomedical field. Mostly, CBNs can be used potentially for medical coatings, drug delivery, medical device fabrication and diagnosis. Graphene and its derivatives still need to explore for their exceptional properties, functionalization and long-term effects.
Compliance with ethical standards
Conflict of interest
The authors declare that they have no competing interests.
- 1.Affatato S, Frigo M, Toni A (2000) An in vitro investigation of diamond-like carbon as a femoral head coating. J Biomed Mater Res Off J Soc Biomater Jpn Soc Biomater Aust Soc Biomater Korean Soc Biomater 53:221–226Google Scholar
- 19.Engelhart S, Segal RJ (2017) Allergic reaction to vanadium causes a diffuse eczematous eruption and titanium alloy orthopedic implant failure. Cutis 99:245Google Scholar
- 23.Ganguly D, Shahbazian-Yassar R, Shokuhfar T (2014) Recent advances in nanotubes for orthopedic implants. J Nanotechnol Smart Mater 1:201Google Scholar
- 24.Gay T, Kaufman J, McGuigan M (2005) Stronger than steel: carbon nanotubes. Boston University, BostonGoogle Scholar
- 26.Ghosh D, Chandra S, Chakraborty A, Ghosh SK, Pramanik P (2010) A novel graphene oxide-para amino benzoic acid nanosheet as effective drug delivery system to treat drug resistant bacteria. Int J Pharm Sci Drug Res 2:127–133Google Scholar
- 32.Hammer P, dos Santos FC, Cerrutti BM, Pulcinelli SH, Santilli CV (2012) Corrosion resistant coatings based on organic–inorganic hybrids reinforced by carbon nanotubes. In: Razavi RS (ed) Recent researches in corrosion evaluation and protection. InTech, RijekaGoogle Scholar
- 40.Inoue S (2014) Multiwalled carbon nanotubes coating accelerates osteoconductivity of anodized titanium [an abstract of dissertation and a summary of dissertation review]Google Scholar
- 45.Kaiser J-P, Krug HF, Wick P (2009) Nanomaterial cell interactions: how do carbon nanotubes affect cell physiology? Future Medicine 4:57–63Google Scholar
- 48.Kamath MS, Ahmed SSSJ, Dhanasekaran M, Santosh SW (2014) Polycaprolactone scaffold engineered for sustained release of resveratrol: therapeutic enhancement in bone tissue engineering. Int J Nanomed 9:183Google Scholar
- 49.Kanayama I et al (2014) Comparative study of bioactivity of collagen scaffolds coated with graphene oxide and reduced graphene oxide. Int J Nanomed 9:3363Google Scholar
- 69.Low KL, Tan SH, Zein SHS, Roether JA, Mouriño V, Boccaccini AR (2010) Calcium phosphate-based composites as injectable bone substitute materials. J Biomed Mater Res Part B Appl Biomater 94:273–286Google Scholar
- 93.Peivandi MT (2013) Exploring the reasons for orthopedic implant failure in traumatic fractures of the lower limb. Arch Iran Med 16:478Google Scholar
- 94.Pramatarova L et al (2007) Artificial bones through nanodiamonds. J Optoelectron Adv Mater 9:236Google Scholar
- 95.Prodana M, Ionita D, Ungureanu C, Bojin D, Demetrescu I (2011) Enhancing antibacterial effect of multiwalled carbon nanotubes using silver nanoparticles. Microscopy 6:549–556Google Scholar
- 99.Rana M, Asim S, Hao B, Yang S, Ma PC (2017) Carbon nanotubes on highly interconnected carbonized cotton for flexible and light-weight energy storage. Adv Sustain Syst 1:10700022Google Scholar
- 103.Sedaghat S, Mehraji M (2013) Novel hybrid of silver nono particles deposited on to the different carbon substrates and evaluation of antibacterial effects. J Appl Sci Eng Technol 3:219–222Google Scholar
- 106.Shepperd JAN, Apthorp H (2005) A contemporary snapshot of the use of hydroxyapatite coating in orthopaedic surgery. Bone Joint J 87:1046–1049Google Scholar
- 109.Suo L et al. (2018) The enhancement of osseointegration using a graphene oxide/chitosan/hydroxyapatite composite coating on titanium fabricated by electrophoretic deposition. J Biomed Mater Res Part B Appl Biomater 106:1–11Google Scholar
- 110.Taeger G, Podleska L, Schmidt B, Ziegler M, Nast-Kolb D (2003) Comparison of diamond-like-carbon and alumina-oxide articulating with polyethylene in total hip arthroplasty. Materialwissenschaft und Werkstofftechnik: Entwicklung Fertigung, Prüfung, Eigenschaften und Anwendungen technischer Werkstoffe 34:1094–1100CrossRefGoogle Scholar
- 111.Tai IC, Fu Y-C, Wang C-K, Chang J-K, Ho M-L (2013) Local delivery of controlled-release simvastatin/PLGA/HAp microspheres enhances bone repair. Int J Nanomed 8:3895Google Scholar
- 113.Tong Y, Bohm S, Song M (2013) Graphene based materials and their composites as coatings. Austin J Nanomed Nanotechnol 1:1003Google Scholar